PRODUCT DATA SHEET
Fontefloor EP 100 - Water-borne epoxy paint
|DESCRIPTION||A two-component water-borne epoxy paint.|
For painting of new, old and earlier painted concrete surfaces. Also suitable for paiting of concrete walls.
|Recommended uses||Recommended for coating of floors exposed to moderate chemical and mechanical stress in industrial facilities, warehouses, repair shops etc.|
|Features||Fontefloor EP 100 belongs to emission class M1 for building materials.|
|Colour Range||RAL, NCS, SSG, BS, MONICOLOR NOVA and SYMPHONY colour cards. AVATINT tinting system.|
|Building material emission class||M1|
Coverage on concrete floors is on the average:
Priming 5–7 m2/l
Finishing 7–10 m2/l
Practical coverage depends on the porosity and evenness of the substrate and on the application method.
|Mixing ratio||Base 3 parts by volume 35V series
Hardener 1 part by volume 008 4571
|Application method||Apply with a rubber trowel and level with a roller.|
|Pot-life (+23°C)||Approx. 50 min after mixing.|
|Drying time at 23°C and 50% relative air humidity||
Dust dry after 6 hours
Recoatable after 16 hours
Fully cured after 7 days
Drying and recoating times are related to the film thickness, temperature, the relative humidity of the air and ventilation.
|Solids volume||approx. 58 %.|
|Density||1.3 kg / l (mixed).|
|Product code||Base paint 35V-s. and hardener 008 4571|
|Application conditions||The relative humidity of the concrete should not exceed 97%. The temperature of the ambient air, surface or coating should not fall below +15ºC during application or drying. Relative humidity of air should not exceed 80 %.|
Remove laitance by power grinding or hydrochloric acid etching. Choose the method best suited for the premises. After grinding remove dust carefully with a vacuum cleaner. Hydrochloric acid etching is carried out with diluted hydrochloric acid (1 part concentrated hydrochloric acid, 4 parts water). Rinse with plenty of water. Dry the floor.
Remove all grease, oil, chemicals and other impurities by MAALIPESU detergent. Remove old peeling paint layer by grinding. Clean out pot-holes removing all loose friable material. Open cracks with e.g. an abrasive tool. Remove loose material and dust.
|Priming||Prime with 25% thinned Fontefloor EP 100 epoxy paint. Add always the water needed to a ready mixture and stir thoroughly. Pour the mixture onto the floor, apply with a rubber trowel and level with a roller.|
|Patching||Fill holes and cracks with a mixture of unthinned Fontefloor EP Primer and dry, clean sand. Mixing ratio e.g. 1 part by volume of Primer mixture and 1–2 parts by volume of sand of grain size 0.1–0.6 mm. Sand the patched areas before finishing.
Note! Concrete surface should always be primed before patching.
|Finishing||Finishing should be done not earlier than 16 hrs after the priming. If the primed surface is not overcoated within 48 hrs, it should be abraded. Thin the paint 25% with water. Pour the mixture onto the floor, apply with a rubber trowel and level with a roller.
The total dry film thickness of the paint film should be approx. 100µm applied in two layers.
For painting of walls thin Fontefloor EP 100 epoxy paint 5–10% with water. Airless spray nozzle tip 0.013" –0.017" and pressure 160–180 bar.
|Mixing of components||First stir base and hardener separately. Mix the correct proportions of base and hardener thoroughly (3–5 minutes) by using a low speed industrial hand drill with a paddle. Insufficient mixing or incorrect mixing ratio will result in uneven drying of the surface, weaken the properties of the coating and risk the success of the application.|
|Cleaning of tools||Equipment should be cleaned immediately after use before the paint has dried.|
|EU VOC 2004/42/EC-limit value||VOC 2004/42/EC (cat A/j) 140 g/l (2010)
|HEALTH AND SAFETY LABELLING|
according to Regulation (EC) No. 1272/2008
|Containers are provided with safety labels, which should be observed. Further information about hazardous influences and protection are detailed in individual health and safety data sheets. A health and safety data sheet is available on request from Tikkurila Oyj.|
|Safety data sheet||Fontefloor EP 100|
|Hardener safety data sheet||Fontefloor EP 100|
|DECLARATION OF PERFORMANCE||Declaration of Performance EN1504-2|
|The European harmonized productstandard EN 1504-2:2004 defines the requirements for surface protection systems for concrete.
This product is tested and CE-labelled in accordance with the tables 1d and 1f in the